||This article needs additional citations for verification. (April 2010)|
Welding Techniques 
A number of techniques are used for welding plastics.
Hot gas welding 
Hot gas welding, also known as hot air welding, is a plastic welding technique using heat. A specially designed heat gun, called a hot air welder, produces a jet of hot air that softens both the parts to be joined and a plastic filler rod, all of which must be of the same or a very similar plastic. (Welding PVC to acrylic is an exception to this rule.)
In the case of webs and films a filler rod may not be used. Two sheets of plastic are heated via a hot gas (or a heating element) and then rolled together. This is a quick welding process and can be performed continuously.
Heat sealing is the process of sealing one thermoplastic to another similar thermoplastic using heat and pressure. The direct contact method of heat sealing utilizes a constantly heated die or sealing bar to apply heat to a specific contact area or path to seal or weld the thermoplastics together. Heat sealing is used for many applications, including heat seal connectors, thermally activated adhesives and film or foil sealing. Common applications for the heat sealing process: Heat seal connectors are used to join LCD displays to PCBs in many consumer electronics, as well as in medical and telecommunication devices. Heat sealing of products with thermal adhesives is used to hold clear display screens onto consumer electronic products and for other sealed thermo-plastic assemblies or devices where heat staking or ultrasonic welding is not an option due to part design requirements or other assembly considerations. Heat sealing also is used in the manufacturing of bloodtest film and filter media for the blood, virus and many other test strip devices used in the medical field today. Laminate foils and films often are heat sealed over the top of thermoplastic medical trays, Microtiter (microwell) plates, bottles and containers to seal and/or prevent contamination for medical test devices, sample collection trays and containers used for food products. Medical and the Food Industries manufacturing Bag or flexible containers use heat sealing for either perimeter welding of the plastic material of the bags and/or for sealing ports and tubes into the bags. A variety of heat sealers are available to join thermoplastic materials such as plastic films: Hot bar sealer, Impulse sealer, etc.
Freehand welding 
With freehand welding, the jet of hot air (or inert gas) from the welder is played on the weld area and the tip of the weld rod at the same time. As the rod softens, it is pushed into the joint and fuses to the parts. This process is slower than most others, but it can be used in almost any situation.
Speed tip welding 
With speed welding, the plastic welder, similar to a soldering iron in appearance and wattage, is fitted with a feed tube for the plastic weld rod. The speed tip heats the rod and the substrate, while at the same time it presses the molten weld rod into position. A bead of softened plastic is laid into the joint, and the parts and weld rod fuse. With some types of plastic such as polypropylene, the melted welding rod must be "mixed" with the semi-melted base material being fabricated or repaired. These welding techniques have been perfected over time and have been utilised for over 50 years by professional plastic fabricators and repairers internationally. Speed tip welding method is a much faster welding technique and with practice can be used in tight corners. A version of the speed tip "gun" is essentially a soldering iron with a broad, flat tip that can be used to melt the weld joint and filler materiel to create a bond.
Extrusion welding 
Extrusion welding allows the application of bigger welds in a single weld pass. It is the preferred technique for joining material over 6 mm thick. Welding rod is drawn into a miniature hand held plastic extruder, plasticized, and forced out of the extruder against the parts being joined, which are softened with a jet of hot air to allow bonding to take place.
Contact welding 
This is the same as spot welding except that heat is supplied with conduction of the pincher tips instead of electrical conduction. Two plastic parts are brought together where heated tips pinch them, melting and joining the parts in the process.
Hot plate welding 
Related to contact welding, this technique is used to weld larger parts, or parts that have a complex weld joint geometry. The two parts to be welded are placed in the tooling attached to the two opposing platens of a press. A hot plate, with a shape that matches the weld joint geometry of the parts to be welded, is moved in position between the two parts. The two opposing platens move the parts into contact with the hot plate until the heat softens the interfaces to the melting point of the plastic. When this condition is achieved the hot plate is removed, and the parts are pressed together and held until the weld joint cools and re-solidifies to create a permanent bond.
The most common form of this welding is butt heat fusion welding which welds two circular tubes end to end.
High frequency welding 
Certain plastics with chemical dipoles, such as PVC, polyamides (PA) and acetates can be heated with high frequency electromagnetic waves. High frequency welding uses this property to soften the plastics for joining. The heating can be localized, and the process can be continuous. Also known as Dielectric Sealing, R.F. (Radio Frequency) Heat Sealing.
In a ferromagnetic work piece, plastics can be induction-welded by formulating them with metallic or ferromagnetic compounds, called susceptors. These susceptors absorb electromagnetic energy from an induction coil, become hot, and lose their heat energy to the surrounding material by thermal conduction.
Radio frequency welding is a very mature technology that has been around since the 1940s. Two pieces of material are placed on a table press that applies pressure to both surface areas. Dies are used to direct the welding process. When the press comes together, high frequency waves (usually 27.12 MHz) are passed through the small area between the die and the table where the weld takes place. This high frequency (radio frequency) field causes the molecules in certain materials to move and get hot, and the combination of this heat under pressure causes the weld to take the shape of the die. RF welding is fast. This type of welding is used to connect polymer films used in a variety of industries where a strong consistent leak-proof seal is required. In the fabrics industry, RF is most often used to weld PVC and polyurethane (PU) coated fabrics. This is a very consistent method of welding.
The most common materials used in RF welding are PVC and polyurethane. It is also possible to weld other polymers such as nylon, PET, EVA and some ABS plastics.
Injection welding 
Injection welding is similar/identical to extrusion welding, except, using certain tips on the handheld welder, one can insert the tip into plastic defect holes of various sizes and patch them from the inside out. The advantage is that no access is needed to the rear of the defect hole. The alternative is a patch, except that the patch can not be sanded flush with the original surrounding plastic to the same thickness. PE and PP are most suitable for this type of process. The Drader injectiweld is an example of such tool.
Ultrasonic welding 
In ultrasonic welding, high frequency (15 kHz to 40 kHz) low amplitude vibration is used to create heat by way of friction between the materials to be joined. The interface of the two parts is specially designed to concentrate the energy for the maximum weld strength. Ultrasonic can be used on almost all plastic material. It is the fastest heat sealing technology available.
Friction welding 
In friction welding, the two parts to be assembled are rubbed together at a lower frequency (typically 100–300 Hz) and higher amplitude (typically 1 to 2 mm (0.039 to 0.079 in)) than ultrasonic welding. The friction caused by the motion combined with the clamping pressure between the two parts creates the heat which begins to melt the contact areas between the two parts. At this point, the plasticized materials begin to form layers that intertwine with one another, which therefore results in a strong weld. At the completion of the vibration motion, the parts remain held together until the weld joint cools and the melted plastic re-solidifies. The friction movement can be linear or orbital, and the joint design of the two parts has to allow this movement.
Spin welding 
Spin welding is a particular form of frictional welding. With this process, one round piece is held stationary, while a mating one is rotated at high velocity while lightly against the stationary piece. The rotated piece is then pressed firmly against the fixed piece. This is a common way of producing low- and medium-duty plastic wheels, e.g., for toys, shopping carts, recycling bins, etc.
Laser welding 
This technique requires one part to be transmissive to a laser beam and either the other part absorptive or a coating at the interface to be absorptive to the beam. The two parts are put under pressure while the laser beam moves along the joining line. The beam passes through the first part and is absorbed by the other one or the coating to generate enough heat to soften the interface creating a permanent weld.
Semiconductor diode lasers are typically used in plastic welding. Wavelengths in the range of 808 nm to 980 nm can be used to join various plastic material combinations. Power levels from less than 1W to 100W are needed depending on the materials, thickness and desired process speed.
Diode laser systems have the following advantages in joining of plastic materials:
- Cleaner than adhesive bonding
- No micro-nozzles to get clogged
- No liquid or fumes to affect surface finish
- No consumables
- Higher throughput
- Can access work-piece in challenging geometry
- High level of process control
Requirements for high strength joints include:
- Adequate transmission through upper layer
- Absorption by lower layer
- Material compatibility – wetting
- Good joint design – clamping pressure, joint area
- Lower power density
A sample list of materials that can be joined include:
For a more in depth list of materials as well as weldable material combinations, please refer to the Laser Plastic Welding Material Compatibility Chart
Specific applications include sealing / welding / joining of: catheter bags, medical containers, automobile remote control keys, heart pacemaker casings, syringe tamper evident joints, headlight or tail-light assemblies, pump housings, and cellular phone parts.
Transparent Laser Plastic Welding
New fiber laser technology allows for the output of higher laser wavelengths, with the best results typically around 2,000 nm, significantly higher than the average 808 nm to 1064 nm diode laser used for traditional laser plastic welding. Because these higher wavelengths are more readily absorbed by thermoplastics than the infra-red radiation of traditional plastic welding, it is possible to weld two clear polymers without any colorants or absorbing additives. Common Applications will mostly fall in the medical industry for devices like catheters and microfluidic devices. The heavy use of transparent plastics, especially flexible polymers like TPU, TPE and PVC, in the medical device industry makes transparent laser welding a natural fit. Also, the process requires no laser absorbing additives or colorants making testing and meeting biocompatibility requirements significantly easier.
Solvent welding 
In solvent welding, a solvent is applied which can temporarily dissolve the polymer at room temperature. When this occurs, the polymer chains are free to move in the liquid and can mingle with other similarly dissolved chains in the other component. Given sufficient time, the solvent will permeate through the polymer and out into the environment, so that the chains lose their mobility. This leaves a solid mass of entangled polymer chains which constitutes a solvent weld.
This technique is commonly used for connecting PVC and ABS pipe, as in household plumbing. The "gluing" together of plastic (polycarbonate, polystyrene or ABS) models is also a solvent welding process.
Dichloromethane (methylene chloride), which is obtainable in paint stripper, can solvent weld polycarbonate and polymethylmethacrylate. Dichloromethane chemically welds certain plastics; for example, it is used to seal the casing of electric meters. It is also a component - along with tetrahydrofuran - of the solvent used to weld plumbing.
Plastic Welding supplies 
Welding rod 
A plastic welding rod, also known as a thermoplastic welding rod, is a rod with circular or triangular cross-section used to bind two pieces of plastic together. They are available in a wide range of colors to match the base material's color.
An important aspect of plastic welding rod design and manufacture is the porosity of the material. A high porosity will lead to air bubbles (known as voids) in the rods, which decrease the quality of the welding. The highest quality of plastic welding rods are therefore those with zero porosity, which are called voidless.
See also 
- Crawford, Lance (January/February 2013 ed.). "Port Sealing: An Effective Heat Sealing Solution". Plastic Decorating Magazine
- "What is High frequency welding". Carmo A/S. Retrieved 16 March 2013.
- "Plastic Welding with Diode Lasers".
- "Material Compatibility Chart for Laser Plastic Welding". Laser Plastic Welding.
- "Potential applications". LPKF Laser & Electronics.
Further reading 
- J. Alex Neumann and Frank J. Bockoff, "Welding of Plastics", 1959, Reinhold publishing.
- Safety in the use of Radiofrequency Dielectric Heaters and Sealers, ISBN 92-2-110333-1
- Michael J. Troughton, "Handbook of Plastics Joining, A Practical Guide", 2nd ed., 2008, ISBN 978-0-8155-1581-4
- Crawford, Lance, "Port Sealing: An Effective Heat Sealing Solution". Plastic Decorating Magazine. January/February 2013 Edition. ISSN 1536-9870. (Topeka, KS: Peterson Publications, Inc.). Section: Assembly: pages 36-39, covers Crawford's article.
- Tres, Paul A., "Designing Plastic Parts for Assembly", 6th ed., 2006, ISBN 978-1-5699-0401-5